Acta Materialia 106 (2016) 144e154
Contents lists available at ScienceDirect
Acta Materialia journal homepage: www.elsevier.com/locate/actamat
Full length article
Grain reﬁning by ultrasonic stirring of the weld pool Tao Yuan a, Sindo Kou b, *, Zhen Luo a a b
School of Materials Science and Engineering, Tianjin University, Tianjin 300072, China Department of Materials Science and Engineering, University of Wisconsin, Madison, WI 53706, USA
a r t i c l e i n f o
a b s t r a c t
Article history: Received 10 October 2015 Received in revised form 4 January 2016 Accepted 8 January 2016 Available online xxx
Grain reﬁning can improve the mechanical properties and solidiﬁcation-cracking resistance of the weld. Ultrasonic grain reﬁning was conducted by dipping an ultrasonic probe in the weld pool to stir it at a distance behind the arc. This new approach produced effective grain reﬁning in arc welds of Mg alloys AZ31 Mg and AZ91 Mg. Grain reﬁning increased when the probe was positioned farther behind the arc. This suggests the initial crystallites or dendrite fragments generated by ultrasound in a cooler melt farther behind the arc were better able to survive. This also suggests dendrite fragmentation was more likely to occur because the probe was closer to the mushy zone. However, a probe too far behind the arc ended up being inside the mushy zone and grain reﬁning, though highly effective, was restricted to only near the weld centerline. At the same probe position, grain reﬁning increased with increasing ultrasound amplitude. Grains were signiﬁcantly ﬁner in AZ91 Mg welds than AZ31 Mg welds. This suggests grain reﬁning increased with increasing constitutional supercooling caused by the higher solute content of AZ91 Mg than AZ31 Mg. © 2016 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.
Keywords: Welding Grain reﬁning Mg alloys Solidiﬁcation Microstructure
1. Introduction Grain reﬁning of welds has been an active area of research in welding because ﬁner grains can improve the strength, ductility and toughness of the weld and increase its resistance to cracking during solidiﬁcation . Numerous techniques for grain reﬁning in welding have been studied, such as arc pulsation [2,3], arc oscillation [3,4], inoculation [5e7], electromagnetic weld-pool stirring [8,9], and ultrasonic weld-pool vibration [10e13]. The approach of using advanced welding power sources for grain reﬁning is attractive because it requires no additional devices to oscillate the arc or stir the pool, nor preparation of special ﬁller metal containing inoculants. For example, in gas-tungsten arc welding He et al.  excited the arc by using high frequency current to generate ultrasonic waves, which caused weld pool vibration and grain reﬁning in welding Tie4Ale4V alloy. For another example, using an advanced gas-tungsten arc welding power source that allowed special AC pulsing, Babu and Cross  grain reﬁned AZ31 Mg welds. Naturally, advanced welding power sources cannot be expected to work in all situations. For instance, the ﬁller metal can interfere with the arc that is set up to generate ultrasonic waves or ﬁne-tuned to pulse
* Corresponding author. E-mail address: [email protected]
(S. Kou). http://dx.doi.org/10.1016/j.actamat.2016.01.016 1359-6454/© 2016 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.
with special current and voltage waveforms. Thus, other approaches to grain reﬁning in welding do have merits. An example is ultrasonic weld pool vibration by mechanical means. Effective grain reﬁning was achieved by ultrasonic vibration of the workpiece in gas-tungsten arc welding of 7075 Al alloy  and in shielded-metal arc welding of 316L stainless steel . The ultrasonic machine in the former was 2 kW in power and 20 kHz in frequency. It was not speciﬁed in the latter, but the use of a 1.5 kW, 20 kHz machine was reported in a related study by the same group . The ultrasonic intensity can be deﬁned as I ¼ rcð2pfAÞ2 =2 (r is the liquid density, c speed of sound in the liquid, f ultrasound frequency and A ultrasound amplitude), and fully developed cavitation can occur in liquid Mg when I 80 W/cm2 . With a very small probe for ultrasonic stirring in a very small volume of liquid in a gas-tungsten arc weld pool, melt wave resistance can be expected to be minimal and a smaller and hence less expensive ultrasonic machine may sufﬁce. Unfortunately, when the workpiece is clamped down tightly to a rigid ﬁxture or connected to a rigid structure, ultrasonic vibration of the workpiece can be difﬁcult. An alternative to overcome this problem was to attach a ﬁller-wire guide to the sonotrode and put the ﬁller wire tip in contact with weld pool edge to transmit ultrasonic waves to the weld pool . The ultrasonic power source was 600 W and 19 kHz. The use of this smaller ultrasonic machine
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
was possible because the wire guide and the weld pool were both very small. This can be another advantage of this approach. Unfortunately, due to its low melting point, the ﬁller wire tip had a tendency to melt, ball up and stop grain reﬁning when moved closer to the arc to improve weld pool vibration. The purpose of the present study was to explore a new approach in which an ultrasonic probe is dipped directly in the weld pool of a Mg alloy and determine how the following factors affect grain reﬁning: 1. the ultrasound amplitude, 2. the distance between the probe and the arc, and 3. the alloy composition. 2. Experimental procedure The experimental approach was to dip an ultrasonic probe, smaller in diameter and much higher in melting point than a ﬁller wire, directly in the weld pool to stir it at a distance behind the arc. This new approach allowed the workpiece to be clamped down tightly as required to avoid distortion induced by welding. It also allowed the probe position in the weld pool to be changed as needed. The ultrasonic probe was a tungsten rod of 0.5 mm diameter (melting point 3407 C). The ﬁne tungsten rod minimized heat extraction from the weld pool. Except for a short section near the weld pool, the rod was inside a 304 stainless steel tube (0.82 mm OD and 0.51 mm ID), and the tube was squeezed (crimped) tight against the rod to stiffen it. The stainless steel tube was mounted on the sonotrode of a STAPLA ultrasonic welding machine, which was available to the authors. The machine was 3 kW, 20 kHz, and the amplitude was adjustable from 14 mm at step one to 28 mm at step ten. The probe vibrated in a horizontal plane in the direction normal to the welding direction. Fig. 1 shows schematically the ultrasonic grain reﬁning process used in the present study. For convenience of subsequent discussion, three possible mechanisms of grain reﬁning are also included. The tip of the ultrasonic probe was dipped in the weld pool from below as illustrated in Fig. 1a. The distance between the probe and the axis of the electrode is called the offset. The workpiece was mounted on a motor-driven carriage that travels in the direction indicated by the arrowhead. The electrode, pool and probe do not travel. The welding torch was mounted on an xey sliding stage driven by precision lead screws that advanced the stage 1 mm per revolution (360 degrees) in either direction. This allowed the horizontal distance between the electrode axis and the probe to be set with a precision much better than 0.1 mm. At the end of welding the arc was turned off abruptly to help preserve the steadyesteady pool shape. The travel of the workpiece was stopped simultaneously. The distance between the probe and the weld pool boundary in the welding direction was measured after welding. The sensitivity of controlling the location of the probe from the pool boundary along the welding direction is estimated to be about ±0.2 mm. In order to investigate the effect of the offset over a wide range, the probe was positioned from 0 to 8 mm behind the electrode axis. After a steady weld pool was established, the sonotrode was raised to dip the probe tip in the weld pool. It is believed that dipping an ultrasonic probe into the weld pool from above, at a short distance behind the arc, is also feasible since the probe is very small. A small water-cooled Cu holder with Ar shielding can be used to protect the probe from the arc. Two commercial Mg alloys were selected for welding, i.e., wrought alloy AZ31 Mg (nominal composition Mge3.0Ale1.0Zne0.6Mn) and casting alloy AZ91 Mg (nominal composition Mge9.0Ale0.7Zne0.2Mn). The workpiece was 102 mm long, 102 mm wide and 1.6 mm thick. It was bead-on-plate welded without a ﬁller metal by gas-tungsten arc welding along the
Fig. 1. Schematic sketches illustrating grain reﬁning during welding: (a) vertical longitudinal cross-section along weld centerline showing ultrasonic stirring of weld pool; (b) horizontal longitudinal cross-section; (c) possible mechanisms of grain reﬁning. In (a) the workpiece alone travels and the direction of travel is indicated by the arrowhead.
centerline of the workpiece top surface. The welding direction was normal to the rolling direction in the case of AZ31 Mg. The welding conditions were as follows: direct current electrode negative, 2%thoriated tungsten electrode 3.2 mm in diameter with a 50 included angle, 1.5 mm arc gap, and pure Ar shielding at 1 m3/h (16.5 L/min). Table 1 summarizes the conditions used for welding and ultrasonic stirring. After welding, the tip of the tungsten probe was easily separated from the weld. No bonding or reaction with Mg was noticed. The resultant welds were cut and their top surfaces polished and etched to reveal the grain structure. The grain structure at the bottom surfaces was also checked, and it was similar to that at the top surfaces. A shallow track was left by the probe at the weld bottom surface, visible with AZ31 Mg but not AZ91 Mg. AZ31 Mg welds were etched with a solution consisting of 3 ml HCl and 100 ml anhydrous ethyl alcohol. This revealed the dendritic structure but not the grain structure. A different etching solution was used, containing 10 ml glacial acetic acid, 10 ml distilled water, 6 g picric acid and 100 ml anhydrous ethyl alcohol, and micrographs were taken with polarized light to show different grains in different colors. No electron back scatter diffraction (EBSD) images were provided to further conﬁrm that the optical micrographs showing grain reﬁning are clear proof of dendrite fragmentation due to ultrasonics instead of due to sectioning effects. However, it should be pointed out that optical micrographs have always been the standard way of studying grain reﬁning and its mechanisms, both in
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
Table 1 Welds made under various conditions of welding and ultrasonic stirring. Amplitude (mm)
Travel speed (mm/s)
1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16
60 60 60 60 60 60 60 60 60 60 60 60 60 60 60 60
5.50 4.23 4.23 4.23 4.23 4.23 4.23 5.50 5.50 5.50 5.50 5.50 5.50 5.50 6.35 6.35
4 0 0 26.44 5 14 5 17.11 5 20.22 5 23.33 6 26.44 no oscillation 4 26.44 5 26.44 6 26.44 7 26.44 8 26.44 no oscillation no oscillation 3 26.44
(13 (10 (10 (10 (10 (10 (10 (13 (13 (13 (13 (13 (13 (13 (15 (15
ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm) ipm)
welding and casting. In fact, optical micrographs were used throughout the many studies cited in the present study, including those on ultrasonic grain reﬁning. As for AZ91 Mg a simple procedure is known to bring out its grain structure very clearly, more effective than polarized light. The commonly used T4 heat treating procedure followed by quenching was used to dissolve the Mg17Al12 phase along grain boundaries (and within grains). This procedure, which allows no grain growth, brings out grain boundaries clearly [16,17]. The heat treated specimens were then polished and etched with a solution of 20 ml glacial acetic acid, 10 ml distilled water, and 100 ml anhydrous ethyl alcohol. Grain size measurements were carried out according to ASTM Standard E112  at different locations within the region of grain reﬁning, where the average grain size is called the reﬁned grain size or simply the grain size. The area fraction of reﬁned grains was calculated by dividing the area of reﬁned grains by that across the entire weld. The microstructure of the welds was also examined by scanning electron microscopy (SEM), with energy dispersive X-ray spectroscopy (EDS) to analyze the compositions of the intermetallic and matrix phases. 3. Results and discussion As mentioned previously, for convenience of discussion three mechanisms of grain reﬁning in welds are illustrated in Fig. 1c, including heterogeneous nucleation, dendrite fragmentation and grain detachment. These mechanisms in aluminum arc welding were discussed by Kou and Le . Heterogeneous nucleation and dendrite fragmentation are well known grain reﬁning mechanisms in welding and casting. Grain detachment, however, may be less well known. Since the workpiece material around the weld pool is heated up to between the liquidus temperature TL and the eutectic temperature TE, it is partially melted. If the partially melted grains carried away by ﬂuid ﬂow survive in the weld pool, they can grow into equiaxed grains to cause grain reﬁning . The results of ultrasonic grain reﬁning are summarized in Table 1. EDS composition analysis showed no detectable tungsten in the weld. This indicates tungsten did not dissolve in the weld pool, consistent with visual inspections that showed no diameter reduction of the tungsten rod after weld pool stirring. An example of the welds is shown in Fig. 2. The probe was pushed into the weld pool when the workpiece had travelled for about 15 mm after the arc was started. As shown, the weld reached a constant width after about 10 mm from its starting point,
Reﬁned grain size (mm) (except #8, 14, 15)
Area fraction of reﬁned grains (%)
0 75 63 63 60 53 52 95 55 51 48 46 31 71 63 34
0 26 28 40 53 70 87 0 86 90 96 100 30 0 0 88
indicating that the steady-state welding condition had been reached. Columnar grains were observed in welds made with the probe immersed in the weld pool but not oscillated during welding. An example is Weld #1 shown in Fig. 3, which was etched with a solution consisting of 3 ml HCl and 100 ml anhydrous ethyl alcohol. Fig. 3a shows the horizontal longitudinal micrograph of the weld, where the dark arrowhead indicates direction of workpiece travel while the white arrowheads indicate the fusion boundary. Long columnar dendrites are visible in the bulk fusion zone. They point inward from the fusion boundary and forward in the welding direction, typical of the columnar grain structure observed in welds made without grain reﬁning. However, columnar dendrites are not visible in the transverse micrograph in Fig. 3b. This is because the transverse cross-section of a columnar dendrite may not necessarily look like one. Fig. 4a and b shows the same weld samples etched with a solution consisting of 20 ml glacial acetic acid, 10 ml distilled water and 100 ml anhydrous ethyl alcohol. These micrographs were taken by polarized light to show the grain structure. The horizontal longitudinal cross-section in Fig. 4a shows columnar grains in the bulk fusion zone. In the transverse micrograph in Fig. 4b columnar grains are clear near the fusion boundary, where they are more or less parallel to the transverse cross-section of the weld. In the bulk fusion zone, however, columnar grains are more or less normal to the transverse cross-section of the weld and thus do not look like columnar grains. Fig. 4c shows the transverse cross-section of a weld (Weld #9) that was made under identical conditions as Weld #1 (Fig. 4a, b) except the probe was oscillated at the amplitude of 26.44 mm. As shown, the grains are equiaxed and much ﬁner than those in Weld #1 made with a still probe. The horizontal longitudinal cross-section of the weld also show ﬁne equiaxed grains (as
Fig. 2. Example of weld macrograph.
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
Fig. 3. Normal optical micrographs of weld # 1: (a) horizontal longitudinal cross-section showing no grain reﬁning at 4 mm offset and 0 mm amplitude; (b) transverse cross-section. White arrowheads: fusion boundaries (weld edges). Dark arrowhead: travel direction of workpiece.
Fig. 4. Polarized-light micrographs of welds: (a) horizontal longitudinal cross-section of weld #1 showing no grain reﬁning at 4 mm offset and 0 mm amplitude; (b) transverse cross-section of weld #1; (c) transverse cross-section of weld #9 showing grain reﬁning by oscillation at 4 mm offset and 26.44 mm amplitude.
will be shown subsequently in Fig. 6b). Thus, grain reﬁning by ultrasonic stirring of the weld pool is conﬁrmed. Optical micrographs of the AZ31 Mg welds are shown in Figs. 5 and 6. In order to explain these results, some mechanisms involved in ultrasonic stirring and grain reﬁning in general [14,20e27] need to be described brieﬂy ﬁrst. According to Abramov et al. , ultrasonic stirring in a liquid metal causes: (i) cavitation, and (ii) acoustic streaming. Cavitation involves the formation, growth, pulsation and collapse of tiny bubbles in the melt, the pressure impulse (compression) of which can be so high that the collapse of
bubbles generates hydraulic shock waves. Acoustic streaming involves bulk ﬂuid ﬂow in the melt, which can vigorously mix the melt, homogenize its temperature, distribute nucleants in the melt, and enhance heat dissipation. According to Ramirez et al. , ultrasonic grain reﬁning can occur by: (i) cavitation-enhanced nucleation, and (ii) cavitationinduced (shock waves) dendrite fragmentation. Cavitationenhanced nucleation can be further interpreted in terms of two different mechanisms: (i) cavitation-induced melting-point elevation, and (ii) cavitation-induced wetting. Cavitation-induced
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
Fig. 5. Polarized-light micrographs showing horizontal longitudinal cross-sections of AZ31 Mg welds and effect of amplitude of ultrasonic stirring on grain structure: (a) 14.00 mm; (b) 17.11 mm; (c) 23.33 mm; (d) 26.44 mm. Offset: 5 mm in (a) through (c) and 6 mm in (d).
melting-point elevation can be explained by the ClausiuseClapyron equation, DTm ¼ TmDPDV/DH, where Tm is the melting point, DP pressure change, DV volume change upon melting, and DH heat of fusion [23,24]. Based on the equation, Ramirez et al.  calculated a melting-point increase of 1.29e6.47 K for a Mg melt under a pressure pulse of 200e1000 atm caused by collapse of cavitation bubbles. The melting-point increase was considered sufﬁcient to activate many of the particles in the melt near the collapsed bubbles. This is because an increase in the melting point is equivalent to increasing undercooling, leading to enhanced nucleation. Cavitation-induced wetting is explained as follows. Cavities and cracks on the surfaces of insoluble particles can be ﬁlled with the melt (that is, wetted by the melt) by the pressure pulse and the wetted particles thus act as effective nucleation sites, leading to enhanced nucleation. According to Liu et al. , a large number of
solid impurity particles, such as the Mn-based intermetallic compounds, exist in the AZ91 melt. By cavitation-induced wetting a portion of these particles can become active nucleants and lead to nucleation upon a slight undercooling, consistent with cooling curves they measured during solidiﬁcation. As for cavitationinduced (shock waves) dendrite fragmentation, Shu et al.  revealed by real-time imaging and analysis that the violent collapse of bubbles can create local shock waves to shatter dendrites nearby into small pieces in a few tens of milliseconds. 3.1. Effect of ultrasound amplitude on grain structure Observation of the weld pool during welding indicated the pool was calm without any signs of turbulence. No signs of probe oscillation could be seen during welding. This is not surprising in
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
Fig. 6. Polarized-light micrographs showing horizontal longitudinal cross-sections of AZ31 Mg welds and effect of probe position (offset) on grain structure: (a) no ultrasonic stirring; (b) 4 mm offset; (c) 7 mm offset; (d) 8 mm offset. Amplitude: 26.44 mm.
view of the very small amplitude of oscillation used, that is, 26.44 mm maximum. This amplitude is much smaller than the pool width, which is about 7 mm wide and 11 mm long. No signiﬁcant difference in the pool shape or size caused by ultrasonic stirring was observed. As shown by AZ31 Mg welds #3 through #7 in Table 1 and Fig. 5, under identical welding conditions and the probe offset, increasing ultrasound amplitude increases grain reﬁning, including reducing the grain size and increasing the area fraction of reﬁned grains. Weld #7 is included for comparison here because its 6 mm offset is fairly close to the 5 mm offset of other welds. In each micrograph the fusion boundary (indicated by an arrow) is near the right side, and the weld centerline is near the left side. In AZ31 Mg weld #3 made at a low amplitude of 14 mm, some equiaxed grains are present along the weld centerline as shown in
Fig. 5a. It is not clear if these equiaxed grains originated from initial crystallites due to cavitation-enhanced nucleation or dendrite fragments due to cavitation-induced dendrite fragmentation. In any case these initial crystallites or dendrite fragments were produced by ultrasonic stirring, and they were not carried far away from the probe probably because ﬂuid ﬂow induced by ultrasonic streaming was weak at low ultrasound amplitude. Consequently, grain reﬁning is limited to near the weld centerline. However, with the amplitude increased to 23.33 mm in weld #6 and 26.44 mm in weld #7, more initial crystallites or dendrite fragments were generated by ultrasonic stirring. Since ﬂuid ﬂow induced by acoustic streaming was faster with higher amplitudes, they were carried farther across of the solidiﬁcation front. Consequently, grain reﬁning occurred in most of the weld as can be seen in Fig. 5c and d.
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
3.2. Effect of probe position on grain structure In order to compare with AZ31 weld #7, weld #2 was made under identical conditions except the offset was changed from 6 mm to 0 mm, that is, from 6 mm behind the arc to directly under it. Surprisingly, grain reﬁning still occurred though limited. The grain size was 75 mm instead of 52 mm as in weld #7, and the area fraction of reﬁned grains was 26% instead of 87%. Due to space limitation the micrograph is not shown here. In order to study the effect of the offset on grain reﬁning a series of welds was made. As shown by AZ31 Mg welds #8 through 13 in Table 1 and Fig. 6, under identical welding conditions and ultrasound amplitude, grain reﬁning increases with increasing offset, up to the solidiﬁcation front. Farther behind the arc the melt is cooler and the initial crystallites generated by cavitation-enhanced nucleation can have a better chance to survive. Meanwhile, an ultrasonic probe farther behind the arc is closer to the mushy zone to cause cavitation-induced dendrite fragmentation. Since the melt is cooler here, and the dendrite fragments can have a better chance to survive. As can be seen in Fig. 6c, with the 7 mm offset weld #12 shows ﬁne grains throughout the weld with an average grain size of 46 mm (Table 1), which is close to that of 52 mm obtained by Babu and Cross  in AZ31 Mg by AC pulsed gas-tungsten arc welding. This grain structure suggests the bulk ﬂuid ﬂow induced by acoustic streaming  appeared strong enough to carry the initial crystallites or dendrite fragments across the entire solidiﬁcation front. In arc welding ﬂuid ﬂow in the weld pool can be driven by gradients of the surface tension along the pool surface. The surface tension of liquid metal tends to decrease with increasing temperature, unless a signiﬁcant amount of a surface-active agent (e.g., sulfur in steel and stainless steel) is present [1,28]. Thus, on the top surface the ﬂow driven by surface-tension gradients is outward from near the arc, where the surface tension is lower due to the higher pool surface temperature, to the pool boundary, where the surface tension is higher due to the lowest pool surface temperature. So, initial crystallites or dendrite fragments near the pool surface may be carried away from the arc to survive near the pool boundary. Fluid ﬂow in an arc weld pool can also be driven by the Lorentz force [1,28]. The force is inward and downward and so is the Lorentz-force-driven ﬂow. This may cause the ﬂow on the top surface to go in the opposite direction of that driven by surfacetension gradients. However, the Lorentz force may not be signiﬁcant in a shallow weld pool under a small welding current of 60 A (weak-Lorentz force). During ultrasonic stirring of the weld pool, the bulk ﬂuid ﬂow induced by acoustic streaming, though the pattern of which is unknown, is likely to dominate over the ﬂow induced either by surface-tension gradients or the Lorentz force. As compared to weld #12, the 95 mm grain size in weld #8 made without ultrasonic grain reﬁning is much larger. Since the grain size is reduced by a factor of about 2 by ultrasonic grain reﬁning, the grain density (i.e., number of grains per unit volume) is increased by a factor of about 23 or 8. Thus, by ultrasonic stirring of the weld pool, the total number of dendrite fragments and initial crystallites that grow into equiaxed grains increases by a factor of about 8. A highly non-uniform weld grain structure was observed when the offset was further increased. AZ31 Mg weld #13 in Fig. 6d was made with the probe moved further from 7 to 8 mm behind the arc. A band of very ﬁne grains of average grain size 31 mm exists along the weld centerline (near the left side of the micrograph), outside which coarse columnar grains still exist. This grain structure suggests the ultrasonic probe was inside the mushy zone. Examination of the position of the weld crater relative to the positions of the probe and the electrode indicated the pool boundary, that is, the solidiﬁcation front, at the weld centerline was about 7.0e7.5 mm
behind the electrode axis during welding. Since the offset was 8 mm, the probe was about 0.5e1.0 mm behind the solidiﬁcation front. Thus, the probe was inside the mushy zone during welding. When surrounded by dendrites, the ultrasonic probe can easily break off their tips into very ﬁne pieces as observed by Shu et al. . Consequently, very ﬁne grains form near the weld centerline. However, since dendrite fragments are inside the mushy zone, they are less likely to be carried by bulk ﬂuid ﬂow to elsewhere along the solidiﬁcation front to form ﬁne equiaxed grains away from the weld centerline. Fig. 7 summarizes the effect of ultrasonic weld pool stirring on grain reﬁning in the AZ31 Mg welds. There is not much grain reﬁning if the offset of the probe and the amplitude of oscillation are both small as illustrated in Fig. 7a. On the other hand, extensive grain reﬁning is possible if the offset and the amplitude are both high. With further increase in the offset, however, the probe can end up being inside the mushy zone. The amplitude of oscillation can be signiﬁcantly reduced by the much higher resistance of the mushy zone to probe oscillation. Furthermore, the dendrite fragments inside the mushy zone cannot be carried by bulk ﬂuid ﬂow to elsewhere along the solidiﬁcation front. Thus, grain reﬁning, though highly effective, is limited to near the centerline of the weld. The equiaxed grains in weld #12 are shown in Fig. 7d. Particles and needles are embedded in the Mg-rich primary solidiﬁcation phase (Mg). EDS analysis showed the particles contained Al but no Mn, thus suggesting they are the g (Mg17Al12) phase. They are likely the divorced eutectic that forms with the eutectic part of the (Mg) phase connected to the primary solidiﬁcation phase (Mg). On the other hand, the needles contained both Al and Mn, thus suggesting they can be an intermetallic compound AlxMny such as Al8Mn5, Al11Mn4 or Al4Mn. There is no clear evidence to prove that heterogeneous nucleation occurred from an AlxMny intermetallic compound. The columnar and equiaxed grains in weld #13 are shown in Fig. 7e and f, respectively. These equiaxed grains are signiﬁcantly ﬁner than those in weld #12 (Fig. 7d). The formation of AlxMny intermetallic compounds during the solidiﬁcation of AZ31 Mg is shown in Fig. 8. For the purpose of comparison, AZ91 Mg is also included. These curves of temperature T vs. fraction solid fS were calculated using the thermodynamic software Pandat  and Mg database PanMagnesium  of CompuTherm, LLC in Madison, WI. According to the curves, Al8Mn5 forms from the melt before the primary Mg-rich phase (Mg) does. In AZ31 Mg, Al8Mn5 forms at 674 C and (Mg) at 632 C. In the case of AZ91 Mg, Al8Mn5 forms at 637 C and (Mg) at 601 C. As mentioned previously, Liu et al.  suggested that by cavitation-induced wetting, some Mn-based intermetallic compounds in the AZ91 melt can become active nucleants. Since solid Al8Mn5 already exists in the melt before (Mg) forms, it is possible for (Mg) to nucleate on solid Al8Mn5 during cooling. However, there is no clear evidence can be seen in Fig. 7d and f that equiaxed grains nucleated from an AlxMny intermetallic compound. In fact, the formation of very ﬁne equiaxed grains along the centerline of weld #13 suggests dendrite fragmentation is likely to be the dominating mechanism of grain reﬁning. The effectiveness of a solid particle in the melt for heterogeneous nucleation is known to depend on the wetting angle of the particle by the melt and the surface roughness of the particle. Low wetting angles (i.e., better extents of wetting) are favored by a low-energy interface between the particle and the solid nucleus, which in turn is favored by a good lattice matching between the particle and the solid. Other factors can also affect the effectiveness, for instance, surface roughness and segregation, and chemical effects . Detachment of partially melted grains may occur and help grain reﬁning, as illustrated in Fig. 1c. This mechanism of grain reﬁning can be more signiﬁcant if the ultrasonic probe is
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
Fig. 7. SEM images showing horizontal longitudinal cross-sections of welds and effect of grain reﬁning: (a) some grain reﬁning with small offset and amplitude; (b) extensive grain reﬁning with large offset and amplitude; (c) probe inside mushy zone due to excessive offset, causing grain reﬁning, though very effective, to be limited to near weld centerline; (d) SEM image of equiaxed grains in weld #12; (e) SEM image of columnar grains in weld #13; (f) SEM image of equiaxed grains in weld #13.
positioned close to the leading portion of the pool boundary. With the probe positioned along the weld centerline, however, grain detachment is less likely to occur. When the offset is increased, the probe is farther away from the partially melted grains. Thus, grain detachment cannot explain why grain reﬁning increases with increasing offset. In casting Ale2Cu with a 18-mm diameter Moealloy sonotrode positioned at the center of the melt surface, Wang et al.  suggested that nucleated grains could also be generated by nucleation, growth and detachments of crystals form the radiating surface of the sonotrode if ultrasonic stirring continued for a period below the liquidus temperature. In the present study, however, the possibility of grain detachment from the sonotrode seems low in view of the very small heat sink provided by the 0.5 mm-diameter sonotrode. In principle, the temperature distribution in the weld pool can be calculated with the probe dipped in the weld pool and this may indicate whether the liquid metal near the probe is locally undercooled. However, this may need considerable numerical modeling, requiring very ﬁne grid spacing around the ﬁne probe to capture the temperature distribution in the nearby liquid. In metal casting the liquid is slightly superheated and there is no external heat source to maintain superheating during solidiﬁcation. Thus, it is possible for solidiﬁcation to occur on a sonotrode as big as 18 mm in diameter to act as a big heat sink. In arc welding, however, the weld pool is highly superheated by the arc continuously . Since the probe is very close to the arc, very small in diameter (0.5 mm) and low in thermal conductivity, it can be expected to be heated above the liquidus temperature of the pool. Thus, it is unlikely that the
liquid near the probe can be undercooled to cause nucleation of grains. This is conﬁrmed by the columnar grains observed in the welds made by dipping the probe in the weld pool without ultrasonic oscillation. No heat transfer analysis was conducted to conﬁrm that the immersion of a very small (0.5 mm diameter) ultrasonic probe in the weld pool cannot cause local undercooling (which, if signiﬁcant, may compete with the dendrite fragmentation due to vibration). However, direct temperature measurements with a thermal probe (i.e., a thermocouple) immersed in the weld pool have indicated no evidence of local undercooling at all. In the ongoing experiments in the welding lab of one of the authors (Kou), a thermocouple of 0.5 mm diameter (the same diameter as the ultrasonic probe) was immersed in the weld pool from the opposite side of the arc at a location behind the arc (the same way the ultrasonic probe was immersed in the weld pool, as shown in Fig. 1a). Instead of local undercooling, local superheating as much as 200 or 300 C was always measured. This is not surprising because the weld pool is so much superheated by the arc that the tip of a very small probe immersed in the pool is superheated by the pool instead of undercooling it. Thus, the mechanism of grain reﬁning is most likely dendrite fragmentation, instead of heterogeneous nucleation or grain detachment. Dendrite fragmentation is most effective if the probe is close to the mushy zone and the amplitude of oscillation is high. Ultrasonic stirring of the weld pool can also signiﬁcantly reduce the temperature gradients in the pool to encourage the dendrite fragments to survive and grow into equiaxed grains.
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
The physical meaning of the growth restriction factor Q can be explained as follows. Based on both equilibrium and nonequilibrium solidiﬁcation, Easton et al.  showed that Q ¼ d(DTc)/d(fS) at fS ¼ 0, where DTc is constitutional supercooling (¼ the equilibrium liquidus temperature minus the actual liquid temperature) and the fS the fraction solid. In other words, Q is the rate of development of constitutional supercooling DTc with respect to the fraction solid fS at the beginning of growth. It was further shown that the growth of a previous grain generates sufﬁcient constitutional supercooling to enable the nucleation event to occur at the next nucleant. The following equation was derived by StJohn et al.  to relate the grain size d to Q:
1 DzDTn ﬃﬃﬃﬃﬃﬃﬃ þ 5:6 d¼p 3 vQ fNv
Fig. 8. Curves of temperature vs. fraction solid showing formation of intermetallic compounds during solidiﬁcation of: (a) AZ31 Mg; (b) AZ91 Mg. The curves were calculated using Pandat  and PanMagnesium  of CompuTherm.
3.3. Effect of alloy composition on grain structure Ultrasonic stirring of the weld pool also caused signiﬁcant grain reﬁning in AZ91 Mg as can be seen in the optical micrographs in Fig. 9. In each micrograph the fusion boundary (indicated by an arrow) is near the right side, and the weld centerline is beyond the left side. The AZ91 Mg welds were wider than the AZ31 Mg welds (mainly because of the lower liquidus temperature of AZ91 Mg) and thus had to be cut off more than one half in order to keep the same photo size as AZ31 Mg. In fact, examination of the micrographs showed ﬁner grains in AZ91 Mg than AZ31 Mg both with and without ultrasonic stirring. The differences can be seen in Table 1 and by comparing Figs. 6 and 9. StJohn et al.  showed that the grain size d measured in castings of Mg alloys can be related to the alloy composition Co as follows:
Q ¼ mL Co ðk 1Þ
where Q: growth restriction factor, mL: slope of the liquidus line of a binary phase diagram, k: equilibrium segregation coefﬁcient. For multi-component alloys with i elements, such as AZ31 Mg and AZ91 Mg,
mLi Coi ðki 1Þ
where f: fraction of particles activated, Nv: number density of particles, D: diffusion coefﬁcient of solute in melt, zDTn: incremental amount of undercooling required for reestablishing the minimum undercooling for nucleation, v: growth rate. The effect of the alloy composition on the grain size in the welds can be explained with the help of Eq. (1) through Eq. (4). First consider the welds made without ultrasonic grain reﬁning. As shown in Table 1, the grain size is 95 mm for AZ31 Mg weld #8 and much ﬁner at 71 mm for AZ91 Mg weld #14. Both welds were made at 5.50 mm/s (13 ipm) travel speed and 60 A current. As shown in Table 2, the growth restriction factor Q is 18.4 C for AZ31 Mg and much larger at 42.7 C for AZ91 Mg. The data for the liquidus slope mL and equilibrium segregation coefﬁcient k were taken from StJohn et al. . Eq. (1) suggests the grain size d decreases with increasing Q. Thus, the smaller grain size in AZ91 Mg weld #14 seems consistent with Eq. (1) if other factors are close. In a recent study by Babu and Cross , AZ31 Mg sheets were butt welded without ultrasonic stirring. Inserts of various Al contents were preplaced between the two sheets to be butt welded together in order to change the weld Al content. The grain size was found to decrease with increasing Al content in the weld. It also decreased with increasing Q, but at high Q values there was a clear negative deviation from linearity. Before leaving the discussion on the AZ91 Mg welds made without ultrasonic grain reﬁning, it is worth mentioning that welds #14 and #15 both show ﬁne equiaxed grains along the fusion boundary, signiﬁcantly ﬁner than those in the bulk weld metal. In fact, AZ31 Mg weld #8 made without ultrasonic grain reﬁning seems to show a similar phenomenon. It is worth noting that Cross et al.  showed that the high undercooling DT associated with the low growth rate  at the fusion boundary can promote nucleation of ﬁne equiaxed grains along the fusion boundary. Now consider the effect of the alloy composition on the grain size in the welds made with ultrasonic grain reﬁning. StJohn et al.  pointed out that in Eq. (4) the fraction of particles activated f is a function of ultrasound amplitude A, that is, f(A). The higher the amplitude A is, the higher f(A) becomes and the smaller the grain size d. As shown in Table 1, the average grain size of AZ91 Mg weld #16 (Fig. 9c) made at 3 mm offset and 26.44 mm amplitude is 34 mm. For comparison, the average grain size of AZ31 Mg weld #12 (Fig. 6c) made at 7 mm offset and 26.44 mm amplitude is 46 mm. It is recognized that the travel speed was 6.35 mm/s for AZ91 Mg weld #16 and 5.50 mm/s for AZ31 Mg weld #12. However, the difference is small. So, AZ91 Mg weld #16 is still signiﬁcantly ﬁner than the AZ31 Mg weld #12 even though the much larger offset of the latter helped grain reﬁning. Thus, as in the case of no ultrasonic stirring, the effect of alloy composition on the grain size through Q is clear.
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
Fig. 9. Normal optical micrographs showing horizontal longitudinal cross-sections of AZ91 Mg welds: (a) no stirring, 5.50 mm/s travel speed; (b) no stirring, 6.35 mm/s travel speed; (c) 26.44 mm amplitude, 3 mm offset, 6.35 mm/s travel speed.
Table 2 Values of Q calculated based on Eq. (3) and mL and k from StJohn et al. . Alloy
Mn (wt %)
Mg (wt %)
Q ( C)
mL ( C/wt%) k AZ31 AZ91
6.87 0.37 3.0 9.0
6.04 0.12 1.0 0.7
1.49 1.10 0.6 0.2
3.4. Effect of travel speed on grain structure Compare AZ31 Mg welds #7 and #11 in Table 1, which were made under identical conditions of welding and ultrasonic stirring except for the travel speed. The former was made at 4.23 mm/s (10 ipm) and the average grain size was 52 mm, while the latter was made at 5.50 mm/s (13 ipm) and the average grain size was 48 mm. Along the centerline of the weld, the travel speed can be considered the same as the growth rate if the effect of the crystal orientation is ignored . The effect of travel speed on the grain size is consistent with Eq. (4) in the sense that the grain size d decreases with increasing growth rate v. However, the effect is not strong. Similar effect of the travel speed can be seen by comparing the two AZ91 Mg welds made without ultrasonic stirring. As shown in Table 1, weld #14 was made at 5.50 mm/s (13 ipm) and the average grain size was 71 mm, while weld #15 was made at 6.35 mm/s (15 ipm) and the average grain size was 63 mm. Again, the effect of travel speed is not strong.
4. Conclusions (1) Effective grain reﬁning can be achieved in welding by ultrasonic stirring of the weld pool with a probe positioned behind the arc, as demonstrated in arc welding of Mg alloys AZ31 Mg and AZ91 Mg. (2) Positioning the probe farther behind the arc can increase grain reﬁning. The initial crystallites or dendrite fragments might have a better chance to survive if they are generated by ultrasonic stirring in a cooler area farther behind the arc. Since a probe farther behind the arc is closer to the mushy zone, it is also more likely to cause dendrite fragmentation. (3) However, a probe too far behind the arc can be inside the mushy zone to cause highly non-uniform grain reﬁning, with extra-ﬁne grains near the weld centerline (where the probe is located) but no grain reﬁning elsewhere in the weld. (4) Grains tend to be signiﬁcantly ﬁner in AZ91 Mg welds than AZ31 Mg welds. And this is true with or without ultrasonic stirring. The higher solute content of AZ91 Mg causes more constitutional supercooling to develop and promotes nucleation. (5) Increasing the ultrasound amplitude increases grain reﬁning. Acknowledgments The authors gratefully acknowledge the support of the National Science Foundation of the United States under Grant No. DMR
T. Yuan et al. / Acta Materialia 106 (2016) 144e154
1500367 and the University of Wisconsin Foundation. The ﬁnancial support by the China Scholarship Council for Tao Yuan to work as a visiting graduate student at UW-Madison is also acknowledged. The authors would like to thank Professor Hongmin Guo of Nanchang University, China, and Jiangwei Liu, Kai Narita, and Tayfun Soysal for their help with the weld microstructure. References  S. Kou, Welding Metallurgy, second ed., John Wiley, Hoboken, New Jersey, 2003.  N.K. Babu, C.E. Cross, Grain reﬁnement of AZ31 magnesium alloy weldments by AC pulsing technique, Metall. Mater. Trans. A 43A (2012) 4145e4154.  S.R.K. Rao, G. Madhusudhana Reddy, M. Kamaraj, K.P. Rao, Grain reﬁnement through arc manipulation techniques in AleCu alloy GTA welds, Mater. Sci. Eng. A 404 (2005) 227e234.  S. Kou, Y. Le, Grain structure and solidiﬁcation cracking in oscillated arc welds of 5052 aluminum alloy, Metall. Trans. A 16A (1985) 1345.  P. Schempp, A. Pittner, M. Rethmeier, Z. Tang, T. Seefeld, C.E. Cross, Inﬂuence of alloy and solidiﬁcation on grain reﬁnement in aluminum weld metal due to inoculation, in Trends in Welding Research, in: Proceedings of the 9th International Conference, June 4-8, ASM International, Chicago, IL, 2012, pp. 98e107, 2013.  S. Sundaresan, G.D. Janaki Ram, R. Murugesan, N. Viswanathan, Combined effect of inoculation and magnetic arc oscillation on microstructure and tensile behaviour of type 2090 AleLi alloy weld fusion zones, Sci. Technol. Weld. Join. 5 (2000) 257.  N.K. Babu, M.K. Talari, D. Pana, Z. Sun, J. Wei, K. Sivaprasad, Microstructural characterization and grain reﬁnement of AA6082 gas tungsten arc welds by scandium modiﬁed ﬁllers, Mater. Chem. Phys. 137 (2012) 543e551.  B.P. Pearce, H.W. Kerr, Grain reﬁnement in magnetically GTA welds of aluminum alloys stirred GTA welds of aluminum alloys, Metall. Trans. B 12B (1981) 479.  F. Matsuda, M. Ushio, H. Nakagawa, K. Nakata, Effects of Electromagnetic Stirring on the Weld Solidiﬁcation Structure of Aluminum Alloys, Arc Physics and Weld Pool Behavior, The Welding Institute, Cambridge, U.K, 1979, pp. 337e347.  L. He, M. Wu, L. Li, H. Hao, Ultrasonic generation by exciting electric arc: a tool for grain reﬁnement in welding process, Appl. Phys. Lett. 89 (2006) 131504.  W. Dai, Effects of high-intensity ultrasonic-wave emission on the weldability of aluminum alloy 7075-T6, Mater. Lett. 57 (2003) 2447e2454.  Y. Cui, C. Xu, Q. Han, Microstructure improvement in weld metal using ultrasonic vibrations, Adv. Eng. Mater. 9 (2007) 161e163.  Y. Cui, C.L. Xu, Q. Han, Effect of ultrasonic vibration on unmixed zone formation, Scr. Mater 55 (2006) 975e978.  G.I. Eskin, Ultrasonic Treatment of Light Alloy Melts, Gordon and Breach, Amsterdam, 1998, pp. 1e25, 135-240.  T. Watanabe, M. Shiroki, A. Yanagisawa, T. Sasaki, Improvement of mechanical properties of ferritic stainless steel weld metal by ultrasonic vibration, J. Mater. Process. Technol. 210 (2010) 1646e1651.  A. Luo, Processing, microstructure, and mechanical behavior of cast magnesium metal matrix composites, Metall. Mater. Trans. A 26A (1995) 2445e2455.
 A. Stevenson, Metals Handbook, 4, ASM International, Materials Park, OH, 1989, p. 899.  ASTM E112, Standard Test Methods for Determining Average Grain Size, ASTM, 2004.  S. Kou, Y. Le, Nucleation mechanisms and grain reﬁning of weld metal, Weld. J. 65 (1986), 305-s.  V. Abramov, O. Abramov, V. Bulgakov, F. Sommer, Solidiﬁcation of aluminum alloys under ultrasonic irradiation using water-cooled resonator, Mater. Lett. 37 (1998) 27e34.  D. Shu, B. Sun, J. Mi, P. Grant, A high-speed imaging and modeling study of dendrite fragmentation caused by ultrasonic cavitation, Metall. Mater. Trans. A 43A (2012) 3755e3765.  J. Li, T. Momono, Y. Fu, Z. Jia, Y. Tayu, Effect of ultrasonic stirring on temperature distribution and grain reﬁnement in Al-1.65%Si alloy melt, Trans, Nonferrous Met. Soc. China 17 (2007) 691e697.  B. Chalmers, Principles of Solidiﬁcation, John Wiley and Sons, New York, 1964.  J. Campbell, Effects of vibration during solidiﬁcation, Int. Met. Rev. 26 (1981) 71e108.  A. Ramirez, M. Qian, B. Davis, T. Wilks, D.H. StJohn, Potency of high-intensity ultrasonic treatment for grain reﬁnement of magnesium alloys, Scr. Mater 59 (2008) 19e22.  X. Liu, Y. Osawa, S. Takamori, T. Mukai, Grain reﬁnement of AZ91 alloy by introducing ultrasonic vibration during solidiﬁcation, Mater. Lett. 62 (2008) 2872e2875.  M. Qian, A. Ramirez, A. Das, D.H. StJohn, The effect of solute on ultrasonic grain reﬁnement of magnesium alloys, J. Cryst. Growth 312 (2010) 2267e2272.  S. Kou, Transport Phenomena and Materials Processing, John Wiley, Hoboken, New Jersey, 1996.  Pandat, Phase Diagram Calculation Software Package for Multicomponent Systems, in: Computherm LLC, Madison,, WI, 2013.  PanMagnesium, Thermodynamic Database for Magnesium Alloys, in: Computherm LLC, Madison,, WI, 2013.  D.A. Porter, K.E. Easterling, M.Y. Sherif, Phase Transformations in Metals and Alloys, third ed., CRC Press, 1980, pp. 188e192.  G. Wang, M.S. Dargusch, M. Qian, D.G. Eskin, D.H. StJohn, The role of ultrasonic treatment in reﬁning the as-cast grain structure during the solidiﬁcation of an Al-2Cu alloy, J. Cryst. Growth 408 (2014) 119e124.  D.H. StJohn, P. Cao, M. Qian, M.A. Easton, A new analytical approach to reveal the mechanisms of grain reﬁnement, Adv. Eng. Mater. 6 (2007) 739e746.  M.A. Easton, D.H. StJohn, A model of grain reﬁnement incorporating alloy constitutional and potency of heterogeneous nucleant particles, Acta Mater. 49 (2001) 1867e1878.  D.H. StJohn, M.A. Easton, M. Qian, J.A. Taylor, Grain reﬁnement of magnesium alloys: A review of recent research, theoretical developments, and their application, Metall. Mater. Trans. A 44A (2013) 2935e2949.  D.H. StJohn, M. Qian, M.A. Easton, P. Cao, Z. Hildebrand, Grain reﬁnement of magnesium alloys, Metall. Mater. Trans. A 36A (2005) 1669e1679.  N.K. Babu, C.E. Cross, Inﬂuence of aluminum content on grain reﬁnement and strength of AZ31 magnesium GTA weld metal, in Trends in Welding Research, in: Proceedings of the 9th International Conference, June 4-8, ASM International, Chicago, IL, 2012, pp. 91e97, 2013.  C.E. Cross, O. Grong, M. Mousavi, A model for equiaxed grain formation along the weld metal fusion line, Scr. Mater. 40 (1999) 1139e1144.  J.D. Hunt, Steady-state columnar and equiaxed growth of dendrites and eutectic, Mater. Sci. Eng. 65 (1984) 75e83.